Journal of Tropical Forest Science 25(4): 497–503 (2013) Mohd Iqbaldin MN et al. PROPERTIES OF COCONUT SHELL ACTIVATED CARBON MN Mohd Iqbaldin1, 2, *, I Khudzir2, MI Mohd Azlan1, AG Zaidi1, B Surani3 & Z Zubri3 1 Universiti Teknologi MARA, 02600 Arau, Perlis, Malaysia Universiti Teknologi MARA, 40450 Shah Alam, Selangor Darul Ehsan, Malaysia 3 SIRIM AMREC Berhad, 09000 Kulim, Kedah, Malaysia 2 Received May 2012 MOHD IQBALDIN MN, KHUDZIR I, MOHD AZLAN MI, ZAIDI AG, SURANI B & ZUBRI Z. 2013. Properties of coconut shell activated carbon. Microwave-induced potassium hydroxide activation was used to produce coconut shell-based activated carbon. Surface area, pore size and specific capacitance value of the carbon produced were analysed to investigate its potential as an electrode material for supercapacitor. The activation process was carried out at 600 W with various irradiation times (10 to 30 min). The activated carbon produced had high surface area ranging from 1244.0–1768.8 m2 g-1 compared with the inactivated carbon, 36.5 m2 g-1. These results were in good agreement with scanning electron micrographs revealing highly porous surface structure. In addition, the specific capacitance value of the material increased from 94.8 to 156.3 F g-1 compared with the inactivated biomass, 6.4 F g-1. The material produced was found to be suitable as an electrode for supercapacitor. Keywords: Chemical activation, electrode, microwave system, supercapacitor MOHD IQBALDIN MN, KHUDZIR I, MOHD AZLAN MI, ZAIDI AG, SURANI B & ZUBRI Z. 2013. Ciriciri karbon teraktif tempurung kelapa. Gelombang mikro digunakan untuk menghasilkan karbon teraktif tempurung kelapa dengan kalium hidroksida sebagai agen pengaktif. Luas permukaan, saiz liang dan nilai kapasiti spesifik karbon yang dihasilkan dianalisis untuk mengkaji potensinya sebagai elektrod kapasitor lampau. Proses pengaktifan dijalankan pada 600 W dengan masa radiasi yang berbeza (10 min hingga 30 min). Karbon teraktif yang dihasilkan mempunyai luas permukaan yang tinggi iaitu antara 1244.0 m2 g-1 dengan 1768.8 m2 g-1 berbanding dengan karbon tak teraktif iaitu 36.5 m2 g-1. Keputusan ini berpadanan dengan keputusan mikrograf imbasan elektron yang menunjukkan struktur permukaan yang poros. Tambahan lagi, nilai kapasiti spesifik bahan teraktif juga meningkat daripada 94.8 F g-1 menjadi 156.3 F g-1 berbanding dengan karbon tak teraktif iaitu 6.4 F g-1. Karbon teraktif yang dihasilkan didapati sesuai sebagai elektrod kapasitor lampau. INTRODUCTION Nowadays, the environmental issue of biomass waste is of top concern. Several researches have been conducted including the production of activated carbon from waste biomass such as date stone (Bouchelta et al. 2008), durian shell (Chandra et al. 2009), soybean oil cake (Tay et al. 2009), cherry stone (Marin et al. 2009), palm shell and coconut shell (Daud & Ali 2004). Activated carbon is a crude form of graphite having porous structure and high surface area (Li et al. 2008). For these reasons, activated carbon is also well suited as an electrode for supercapacitor. The porous structure of activated carbon is important for ion to migrate and occupy the pores of carbon repetitively to form layers at the interface of electrode–electrolyte in *[email protected] © Forest Research Institute Malaysia 497 electrochemical energy-storage devices (Pandolfo & Hollenkamp 2005). There are two types of activation processes to produce activated carbon from carbonaceous materials, i.e. chemical and physical activation processes. Physical activation procedure involves a two-step process, i.e. carbonisation, followed by activation using steam, oxygen or carbon dioxide as an activating agent (Yuen & Hameed 2009). However, in the chemical activation procedure, carbonisation and activation processes occur in a single stage using chemicals as an activating agent such as potassium hydroxide (KOH), phosphoric acid and zinc chloride (Ncibi et al. 2009). The production of activated carbon from coconut shell using microwave was done by Li Journal of Tropical Forest Science 25(4): 497–503 (2013) Mohd Iqbaldin MN et al. et al. (2009) and Yang et al. (2010). However, there were differences between their study and this study because they used a physical activation process which provided different activating agent and longer time. Our study focused on the application of activated carbon for supercapacitor electrode. However, the activated carbon obtained from their study had high specific surface area with pore structure falling in the range of micropores, rendering it unsuitable as supercapacitor electrode. Supercapacitor is attracting attention nowadays owing to its capability in storing more energy, high power discharge ability and longer life cycle compared with other available energystorage devices (Yuan et al. 2005). Supercapacitor electrode is one of the activated carbon used in electronic industry. Supercapacitor can provide high power capability (60–120 s), excellent reversibility (90–95% or higher) and long life cycle (> 105) (Zhang et al. 2009). In a supercapacitor, the activated carbon used must have porous texture which is the main criterion of a double electric layer with high capacity and charge exchange. The pore structure of the activated carbon used is important for optimal performance of carbon materials as an electrode for supercapacitor (Babel & Jurewicz 2004). In this study, the microwave carbonisation irradiation system was used to produce coconut shell activated carbon (CSAC) using KOH as an activating agent. The properties of the activated material such as surface area, pore size and specific capacitance value were analysed to study the potential of the material for supercapacitor electrode. in an oven at 80 °C. The raw material was ground and sieved into sizes of less than 2 mm to ensure that they were thoroughly mixed with activating agent during the impregnation process. The proximate and ultimate analyses of raw materials were measured using thermal gravimetric analyser and elemental analyser respectively. The particles of coconut shell were then added to 50% KOH (85% purity in a ratio of 1 g of precursor per 0.75 mL of solution) (Deng et al. 2010). The impregnated sample was heated using a microwave oven at 600 W at various irradiation times (10, 15, 20, 25 and 30 min) (Li et al. 2008). The heated process occurred in the presence of nitrogen gas (100 ml min-1) (Marin et al. 2009). The nitrogen gas used was 98% pure. Figure 1 shows the microwave irradiation system used. A modified probe was used to monitor the activation temperature of the activation process. The irradiated sample that became lumpy was washed using 50% hydrochloric acid and water with pH 6.5–7.0 to remove excess KOH. The sample was then dried in an oven at 100 °C for 2 hours. Characterisation of the activated carbon The pore size and structure of the activated carbon were determined using N2 adsorption Brunauer-Emmett-Teller (BET) and scanning electron microscope (SEM) respectively. Samples for the SEM were prepared by cutting the dried samples to fit the specimen stub. The sample surface was sputter coated with a thin film of platinum before being viewed using SEM (Chandra et al. 2009). Adsorption was performed at -196.2 °C using an automatic volumetric sorption analyser and by immersion calorimetry at 19.9 °C (Marin et al. 2009). The surface area and pore size of CSAC produced were determined using the BET analysis software. The BET surface area was MATERIALS AND METHODS Preparation of activated carbon The coconut shells were collected, washed with distilled water and dried overnight Condenser Probe N2 inlet Crucible N2 flow measurement Figure 1 © Forest Research Institute Malaysia Volatile sample collection Pump Sample Microwave Illustration of the operational system for this study 498 Journal of Tropical Forest Science 25(4): 497–503 (2013) Mohd Iqbaldin MN et al. measured by means of standard BET equation applied with relative pressure (P/P0) ranging from 0.06 to 0.30. Electrochemical measurements The cyclic voltammetry test was used to estimate specific capacitance value. The unit was expressed in Farads per mass (F g-1) of carbon material. The CSAC electrodes were soaked in 10 M KOH of electrolyte for 2 hours and these symmetric electrodes were sandwiched with separators using Teflon cell before undergoing cyclic voltammetry test. The symmetric electrodes of CSAC were tested at 0–1 V with scan rate of 2 mV s -1 in aqueous electrolyte (10 M KOH). RESULTS AND DISCUSSION Table 1 shows that waste coconut shell material is a carbonaceous material that has high composition of carbon and high potential to become activated carbon. The percentage of carbon significantly increased after carbonisation and activation process to become CSAC. Textural characteristics of the coconut shellbased activated carbon The SEM micrographs of coconut shell carbon (CSC) and CSAC showed large differences in surface morphology (Figure 2). During carbonisation, most volatile matter was released. However, no pores developed due to the absence of an activating agent. In CSAC, however, hollow pits were observed and these were due to the Table 1 loss of volatile matter and the effect of KOH activating agent on the carbon material (Wang et al. 2009). According to the International Union of Pure and Applied Chemistry, the pore development of an activated carbon is classified into three groups which are micropores (size < 2 nm), mesopores (2–50 nm) and macropores (size > 50 nm) (Pandolfo & Hollenkamp 2005). Apparently, the detected activation temperature of the process increased significantly with increasing irradiation time (Table 2). The surface area of the CSAC was higher than CSC. Chemical activation had increased the porosity of the surface area of CSAC up to 1768.8 m 2 g -1 compared with CSC at only 36.5 m2 g-1. This indicates that the activation process has successfully increased the surface area and porosity of char derivative from carbonised organic precursor (Marin et al. 2009). Table 2 also reveals that time has significant influence on the activation process. The surface area of CSAC increased from 1244.0 to a maximum of 1768.8 m 2 g -1. The pore size of CSAC slightly increased from 2.3 to 2.7 nm with increasing irradiation time from 10 to 20 min. As the irradiation time increased to 30 min, the detected activation temperature also increased, resulting in decreasing surface area of CSAC from 1768.8 to 1399.8 m2 g-1. However, the pore size of CSAC slightly increased from 2.7 to 2.9 nm due to the sintering process which destroyed and widened the pore during the process (Yuen & Hameed 2012). This observation can be explained by two factors that affect the pore development of the carbon material. Proximate and ultimate analyses of coconut shell (CS), coconut shell carbon (CSC) and coconut shell activated carbon (CSAC) Analysis Proximate Volatile matter Fixed carbon Ash content Ultimate Carbon Hydrogen Nitrogen Sulphur Oxygena CS CSC 77.82 21.38 0.8 48.25 50.55 1.20 28.46 69.49 2.05 49.62 7.31 0.22 0.10 42.75 64.87 4.66 0.84 0.09 29.54 80.13 2.36 1.10 0.06 16.35 a Calculated by difference after all elements were determined © Forest Research Institute Malaysia 499 CSAC Journal of Tropical Forest Science 25(4): 497–503 (2013) Mohd Iqbaldin MN et al. (a) (b) Figure 2 SEM micrographs of (a) coconut shell carbon and (b) coconut shell activated carbon (1)When the irradiation time is above 20 min, the activation reaction is over because the activating agent is used up. This means that the ratio of KOH used also has an influence on pore development during the activation process. This phenomenon of the activation process is found similar to a previous study (Yongbin et al. 2007). (2)The increasing irradiation time causes the activation temperature to increase significantly. Pores are formed and destructed simultaneously during the activating period (Liu et al. 2010). At certain activation temperature, activation reaction between KOH and carbon within © Forest Research Institute Malaysia 500 the sample increases which promotes more pore formation, hence increasing the surface area of CSAC. However, when the activation temperature reaches its limit, the destruction of the pore formation becomes dominant and consequently decreases the surface area. Hence, pore size becomes wider from micropores to mesopores (Yongbin et al. 2007). Specific capacitance determination Highly porous electrodes with very high surface area are important for a supercapacitor. Increasing surface area of carbon material Journal of Tropical Forest Science 25(4): 497–503 (2013) Table 2 Mohd Iqbaldin MN et al. Surface area and pore size of coconut shell carbon (CSC) and coconut shell activated carbon (CSAC) with different microwave radiation times Detected temperature (°C) Surface area (m2 g-1) Pore size (nm) CSAC 10 min 530 1244.0 2.3 CSAC 15 min 577 1311.1 2.5 CSAC 20 min 635 1768.8 2.7 CSAC 25 min 702 1536.2 2.8 CSAC 30 min 744 1399.8 2.9 CSC 20 min 399 36.5 3.7 Sample (Time) generally leads to increasing specific capacitance value of the material. The specific capacitance (Csp) of electrodes can be measured using the equation (Yuan et al. 2005) below. Table 3 Csp of coconut shell carbon (CSC) and coconut shell activated carbon (CSAC) with different microwave radiation times Csp = (|Ia| + |Ic|) / (2W dv/dt) where the average of anodic (Ia) and cathodic (Ic) currents is divided by scan rate (dv/dt) and mass of active material (W). Table 3 shows the Csp values of CSAC (at different irradiation times) and CSC which indicate a large difference in specific capacitance of the former (156.33 F g -1 ) and the latter (6.42 F g-1). Large difference in C sp between the two materials showed that high surface area gave positive impact on Csp (Yuan et al. 2005). The pore formation is very important for ion migration. It is also important for ions to occupy all pores of the carbon repetitively forming layers at the interface of electrode–electrolyte. Hence, accumulation of ions during charging will increase, thus, the increase in specific capacitance of the material (Pandolfo & Hollenkamp 2005). Figure 3 shows cyclic voltammogram curves for CSAC and CSC, indicating the difference in specific capacitance of the two materials as electrode materials. The CSAC exhibited higher charge–discharge curve profile than the CSC. The curve profile occurred reversibly without having any influence from Faradic scans. This indicates that the charge separation occurs electrostatically at the interface of electrode– electrolyte. Table 3 indicates the difference in specific capacitance with different irradiation times. The specific capacitance of CSAC increased from 94.77 to 156.33 F g-1 with increasing irradiation time from 10 to 20 min. However, beyond 20 min of irradiation time, the specific capacitance © Forest Research Institute Malaysia 501 Sample (Time) Specific capacitance, Csp (F g-1) CSAC (10 min) 94.77 CSAC (15 min) 101.01 CSAC (20 min) 156.33 CSAC (25 min) 136.18 CSAC (30 min) 113.53 CSC (20 min) 6.42 decreased for CSAC 25 min and CSAC 30 min samples with values of 136.18 and 113.53 F g-1 respectively. The cyclic voltammogram curves of CSAC at different irradiation times (Figure 4) indicated that the sample of CSAC 20 min had the largest rectangular shape behaviour while the sample of CSAC 10 min, the smallest. This shows that by increasing the irradiation time, the specific capacitance of the activated carbon increases (up to certain irradiation time) because of the increasing surface area and pore size. In fact, this phenomenon happens because of the effect of the surface area and pore size of the materials. These are important for ions to migrate and occupy all pores of carbon repetitively. This process will form layers at the interface of electrode–electrolyte (Pandolfo & Hollenkamp 2005). The higher the specific capacitance, the larger the amount of electric charge stored in carbon, resulting in high energy density. It could be deduced that CSAC had higher specific capacitance due to increasing ion accumulation at the interface of electrode–electrolyte compared with the raw and CSC materials. Journal of Tropical Forest Science 25(4): 497–503 (2013) Mohd Iqbaldin MN et al. 3.2 2.4 CSAC Current (mA) 1.6 0.8 0.0 CSC -0.8 -0.6 -2.4 -3.2 0.0 0.2 0.4 0.6 0.8 Voltage (V) Figure 3 Cyclic voltammogram curves of coconut shell activated carbon (CSAC) and coconut shell carbon (CSC) 6 Current (mA) 4 2 -0 -2 -4 -6 CSAC 30 min CSAC 25 min 0.0 0.2 CSAC 20 min CSAC 15 min 0.4 CSAC 10 min 0.6 0.8 Voltage (V) Figure 4 Cyclic voltammogram curves of the coconut shell activated carbon (CSAC) with different activation times of 10 to 30 min Interestingly, the specific capacitance of the CSAC that was produced using microwave irradiation carbonisation system seemed to be comparable with others. Fuertes et al. (2009) prepared activated carbon from mesostructured SBA-16 silica materials using polyfurfuryl alcohol as a carbon precursor. The surface area of the activated carbon ranged from 1500 to 1800 m2 g-1 and pore size ranged from 2 to 8 nm. Specific capacitance of the activated carbon ranged from 100 to 150 F g -1 . The © Forest Research Institute Malaysia 502 activated carbon showed similar characteristics to CSAC. However, Zhang et al. (2009) reported that activated carbon had specific capacitance of 40 F g -1. Merino et al. (2005) reported that industrial activated carbon nanofibres produced by Grupo Antolin Ingenieria SA at an industrial scale had specific capacitance ranging from 50 to 60 F g-1. Thus, it is proven that specific capacitance of CSAC produced within the microwave system is comparable with and has potential to be an electrode material for supercapacitor. Journal of Tropical Forest Science 25(4): 497–503 (2013) Mohd Iqbaldin MN et al. CONCLUSIONS KOH activation of coconut shell via microwave at 600 W and 20 min activation time seemed to be effective in producing carbon material with large surface area (1768.8 m2 g-1) and porosity (2.7 nm) accessible to electrolyte ions. The activation process produced the largest surface area of CSAC, which led to the highest specific capacitance at low current density (156.33 F g-1 in 10 M KOH). ACKNOWLEDGEMENTS The authors gratefully acknowledge the financial support from Universiti Teknologi MARA and collaboration with SIRIM AMREC Berhad. The authors also thank all project members for support and collaboration. REFERENCES Babel K & Jurewicz K. 2004. KOH activated carbon fabrics as supercapacitor material. Journal of Physical and Chemical Solids 65: 275–280. Bouchelta C, Medjram MS, Bertrand O & Bellat JP. 2008. Preparation and characterization of activated carbon from date stones by physical activation with steam. Journal of Analysis Applied Pyrolysis 82: 70–77. Chandra TC, Mirna MM, Sunarso J, Sudaryanto Y & Ismadji S. 2009. Activated carbon from durian shell: preparation and characterization. Journal of Taiwan Institute Chemical Engineering 40: 457–462. D aud WMAW & A li WSW. 2004. Comparison on pore development of activated carbon produced from palm shell and coconut shell. Bioresource Technology 93: 63–69. D eng H, L i G, Y ang H & T ang J. 2010. Preparation of activated carbons from cotton stalk by microwave assisted KOH and K 2 CO 3 activation. Chemical Engineering Journal 163: 373–381. Fuertes AB, Lota G, Centeno TA & Frackowiak E. 2009. Templated mesoporous carbon for supercapacitor application. Electrochimical Acta 50: 2799–2805. Li W, Peng J, Zhang L, Yang K, Xia H, Zhang S & Guo SH. 2009. Preparation of activated carbon from coconut shell chars in pilot-scale microwave heating equipment at 60 kW. Waste Management 29: 756–760. Li W, Zhang LB, Peng JH, Li N & Zhu XY. 2008. Preparation of high surface area activated carbons from tobacco stems with K 2 CO 3 activation using microwave radiation. Industrial Crops and Products 27: 341–347. © Forest Research Institute Malaysia 503 Liu QS, Zheng T, Wang P & Guo L. 2010. Preparation and characterization of activated carbon from bamboo by microwave-induced phosphoric acid activation. Industrial Crops and Products 31: 233–238. Marín MO, Fernández JA, Lázaro MJ, Fernández-González C, Macías-García A, Gómez-Serrano V, Stoeckli F & Centeno TA. 2009. Cherry stones as precursor of activated carbons for supercapacitors. Material, Chemical and Physical 114: 323–327. Merino C, Soto P, Vilaplana-Ortego E, Gomez De Salazar JM, Pico F & Rojo JM. 2005. Carbon nanofibres and activated carbon nanofibres as electrodes in supercapacitors. Carbon 43: 551–557. Ncibi MC, Jeanne-Rose V, Mahjoub B, Jean-Marius C, Lambert J, Ehrhardt JJ, Bercion Y, Seffen M & Gaspard S. 2009. Preparation and characterization of raw chars and physically activated carbons derived from marine Posidonia oceanica (L.) fibres. Journal of Hazardous Material 165: 240–249. Pandolfo AG & Hollenkamp AF. 2005. Carbon properties and their role in supercapacitors. Journal of Power Sources 157: 11–27. T ay T, U car S & K aragöz S. 2009. Preparation and characterization of activated carbon from waste biomass. Journal of Hazardous Material 165: 481–485. W a n g T, T a n S & L i a n g C. 2009. Preparation and characterization of activated carbon from wood via microwave-induced ZnCl2 activation. Carbon 47: 1867–1885. Yang K, Peng J, Srinivasakannan C, Zhang L, Xia H & Duan X. 2010. Preparation of high surface area activated carbon from coconut shells using microwave heating. Bioresource Technology 101: 6163–6169. Yongbin J, Li T, Zhu L, Wang X & Lin Q. 2007. Preparation and characterization of activated carbon by microwave heating KOH activation. Applied Surface Science 254: 506–512. Y u a n GH, J i a n g ZH, A r a m at M & G a o YZ. 2005. Electrochemical behavior of activated-carbon capacitor material loaded with nickel oxide. Carbon 43: 2913–2917. Yuen FK & Hameed BH. 2009. Recent developments in the preparation and regeneration of activated carbons by microwaves. Advance in Colloid and Interface Science 149: 19–27. Yuen FK & Hameed BH. 2012. Coconut husk derived activated carbon via microwave induced activation: effects of activation agents, preparation parameters and adsorption performance. Chemical Engineering Journal 184: 57–65. Zhang Y, Feng H, Wu X, Wang L, Zhang A, Xia T, Dong H, Li X & Zhang L. 2009. Progress of electrochemical capacitor electrode materials: a review. International Journal of Hydrogen Energy 34: 4889–4899.